LMucko/crystallography-open-database huggingface dataset:
Neue ternaere Calcium- und Ytterbium-Silber-Aluminide mit unterschiedlich gestapelten Silber-Aluminium-Kagome-Netzen
Geibel, C.; Mehner, A.; Henseleit, R.; Czech, E.; Roehr, C.; Cordier, G.; Thies, S.; Doersam, G.; Journal of the Less-Common Metals 169 (1991) 55–72; doi:10.1016/0022-5088(91)90235-V

data_1509575
_publ_section_title
;
 Neue ternaere Calcium- und Ytterbium-Silber-Aluminide mit unterschiedlich
 gestapelten Silber-Aluminium-Kagome-Netzen
;
_journal_name_full               'Journal of the Less-Common Metals'
_journal_page_first              55
_journal_page_last               72
_journal_paper_doi               10.1016/0022-5088(91)90235-V
_journal_volume                  169
_journal_year                    1991
_chemical_formula_sum            'Ag1.04933 Al1.95067 Pr'
_chemical_name_systematic        'Ag Al2 Pr'
_space_group_IT_number           166
_symmetry_space_group_name_Hall  '-R 3 2"'
_symmetry_space_group_name_H-M   'R -3 m :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            9
_cell_length_a                   5.632
_cell_length_b                   5.632
_cell_length_c                   27.045
_cell_volume                     742.921
_citation_journal_id_ASTM        JCOMAH
_cod_data_source_file            silver1-2_573.cif
_cod_data_source_block           Ag1.04933Al1.95067Pr1
_cod_original_cell_volume        742.9214
_cod_original_formula_sum        'Ag1.04933 Al1.95067 Pr1'
_cod_database_code               1509575
Synthesis and Crystal Structures of REAgMg (RE = La, Ce, Nd, Eu, Gd, Tb, Ho, Tm, and Yb)
Fickenscher, T.; Poettgen, R.; Journal of Solid State Chemistry 161 (2001) 67–72; doi:10.1006/jssc.2001.9268

data_1509576
_publ_section_title
;
 Synthesis and Crystal Structures of REAgMg (RE = La, Ce, Nd, Eu, Gd, Tb,
 Ho, Tm, and Yb)
;
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              67
_journal_page_last               72
_journal_paper_doi               10.1006/jssc.2001.9268
_journal_volume                  161
_journal_year                    2001
_chemical_formula_sum            'Ag1.053 Mg0.947 Yb'
_chemical_name_systematic        'Yb Ag Mg'
_space_group_IT_number           62
_symmetry_space_group_name_Hall  '-P 2ac 2n'
_symmetry_space_group_name_H-M   'P n m a'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   7.5366
_cell_length_b                   4.4649
_cell_length_c                   8.872
_cell_volume                     298.544
_citation_journal_id_ASTM        JSSCBI
_cod_data_source_file            silver1-2_574.cif
_cod_data_source_block           Ag1.053Mg0.947Yb1
_cod_original_cell_volume        298.5443
_cod_original_formula_sum        'Ag1.053 Mg0.947 Yb1'
_cod_database_code               1509576
Structure and Properties of GdTMg (T = Pd, Ag, Pt)
Hoffmann, R.D.; Tomkowicz, Z.; Pacyna, A.; Fickenscher, T.; Mishra, R.; Piotrowski, H.; Poettgen, R.; Kmiec, R.; Latka, K.; Journal of Solid State Chemistry 168 (2002) 331–342; doi:10.1006/jssc.2002.9718

data_1509577
_publ_section_title
;
 Structure and Properties of GdTMg (T = Pd, Ag, Pt)
;
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              331
_journal_page_last               342
_journal_paper_doi               10.1006/jssc.2002.9718
_journal_volume                  168
_journal_year                    2002
_chemical_formula_sum            'Ag1.062 Gd Mg0.939'
_chemical_name_systematic        'Gd Ag1.062 Mg0.939'
_space_group_IT_number           189
_symmetry_space_group_name_Hall  'P -6 -2'
_symmetry_space_group_name_H-M   'P -6 2 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            3
_cell_length_a                   7.68
_cell_length_b                   7.68
_cell_length_c                   4.1992
_cell_volume                     214.496
_citation_journal_id_ASTM        JSSCBI
_cod_data_source_file            silver1-2_575.cif
_cod_data_source_block           Ag1.062Gd1Mg0.939
_cod_original_cell_volume        214.4962
_cod_original_formula_sum        'Ag1.062 Gd1 Mg0.939'
_cod_database_code               1509577
Crystal structure of cerium silver phosphide (1:1.08:1.90), Ce Ag1.08 P1.90
Demchyna, R.O.; Kuz'ma, Yu.B.; Grin', Yu.; Chikhrii, S.I.; Borrmann, H.; Zeitschrift fuer Kristallographie - New Crystal Structures 217 (2002) 161–162; doi:

data_8103401
_publ_section_title
;
 Crystal structure of cerium silver phosphide (1:1.08:1.90), Ce Ag1.08
 P1.90
;
_journal_name_full
;
Zeitschrift fuer Kristallographie - New Crystal Structures
;
_journal_page_first              161
_journal_page_last               162
_journal_volume                  217
_journal_year                    2002
_chemical_formula_sum            'Ag1.08 Ce P1.9'
_chemical_name_systematic        'Ce Ag1.08 P1.9'
_space_group_IT_number           139
_symmetry_space_group_name_Hall  '-I 4 2'
_symmetry_space_group_name_H-M   'I 4/m m m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   4.0037
_cell_length_b                   4.0037
_cell_length_c                   20.435
_cell_volume                     327.565
_citation_journal_id_ASTM        ZKNSFT
_cod_data_source_file            silver1-2_576.cif
_cod_data_source_block           Ag1.08Ce1P1.9
_cod_original_cell_volume        327.5651
_cod_original_formula_sum        'Ag1.08 Ce1 P1.9'
_cod_database_code               8103401
_cod_duplicate_entry 8100664
New Ln (Ag, Al)4 (Ln= Y, Gd, Tb, Dy) intermetallics and their structure
Kuz'ma, Yu.B.; Stel'makhovich, B.M.; Izvestiya Akademii Nauk SSSR, Metally 1990 (1990) 209–211; doi:

data_1509578
_publ_section_title
;
 New Ln (Ag, Al)4 (Ln= Y, Gd, Tb, Dy) intermetallics and their structure
;
_journal_name_full               'Izvestiya Akademii Nauk SSSR, Metally'
_journal_page_first              209
_journal_page_last               211
_journal_volume                  1990
_journal_year                    1990
_chemical_formula_sum            'Ag1.1 Al6.9 Dy2'
_space_group_IT_number           71
_symmetry_space_group_name_Hall  '-I 2 2'
_symmetry_space_group_name_H-M   'I m m m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            1
_cell_length_a                   4.296
_cell_length_b                   4.179
_cell_length_c                   9.995
_cell_volume                     179.440
_citation_journal_id_ASTM        IZNMAQ
_cod_data_source_file            silver1-2_577.cif
_cod_data_source_block           Ag1.1Al6.9Dy2
_cod_original_cell_volume        179.4401
_cod_database_code               1509578
Para-Schachnerite, Ag1.2 Hg.8, und Schachnerit, Ag1.1 Hg.9, vom Landsberg bei Obermoschel, Pfalz
Muecke, A.; Seeliger, E.; Neues Jahrbuch fuer Mineralogie. Abhandlungen (Band-Nr) (1950-) 117 (1972) 1–18; doi:

data_1509579
_publ_section_title
;
 Para-Schachnerite, Ag1.2 Hg.8, und Schachnerit, Ag1.1 Hg.9, vom Landsberg
 bei Obermoschel, Pfalz
;
_journal_name_full
;
Neues Jahrbuch fuer Mineralogie. Abhandlungen (Band-Nr) (1950-)
;
_journal_page_first              1
_journal_page_last               18
_journal_volume                  117
_journal_year                    1972
_chemical_formula_sum            'Ag1.1 Hg0.9'
_space_group_IT_number           194
_symmetry_space_group_name_Hall  '-P 6c 2c'
_symmetry_space_group_name_H-M   'P 63/m m c'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            1
_cell_length_a                   2.978
_cell_length_b                   2.978
_cell_length_c                   4.843
_cell_volume                     37.196
_citation_journal_id_ASTM        NJMIAK
_cod_data_source_file            silver1-2_578.cif
_cod_data_source_block           Ag1.1Hg0.9
_cod_original_cell_volume        37.19585
_cod_database_code               1509579
Lattice spacing relationships and the electronic structure of hcp zeta phases based on silver
King, H.W.; Massalski, T.B.; Philosophical Magazine, Serie 6 (1901-1925) 6 (1961) 669–682; doi:

data_1509580
_publ_section_title
;
 Lattice spacing relationships and the electronic structure of hcp zeta
 phases based on silver
;
_journal_name_full               'Philosophical Magazine, Serie 6 (1901-1925)'
_journal_page_first              669
_journal_page_last               682
_journal_volume                  6
_journal_year                    1961
_chemical_formula_sum            'Ag1.1 Hg0.9'
_chemical_name_systematic        '(Ag11 Hg9)0.1'
_space_group_IT_number           194
_symmetry_space_group_name_Hall  '-P 6c 2c'
_symmetry_space_group_name_H-M   'P 63/m m c'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            1
_cell_length_a                   2.9896
_cell_length_b                   2.9896
_cell_length_c                   4.8413
_cell_volume                     37.473
_citation_journal_id_ASTM        PHMAA4
_cod_data_source_file            silver1-2_579.cif
_cod_data_source_block           Ag1.1Hg0.9
_cod_original_cell_volume        37.47303
_cod_database_code               1509580
A single-crystal x-ray diffraction study of the ion exchange of Cd2+ into Ag+ beta-alumina
Farrington, G.C.; Edstroem, K.; Thomas, J.O.; Acta Crystallographica B (39,1983-) 47 (1991) 643–650; doi:

data_2105353
_publ_section_title
;
 A single-crystal x-ray diffraction study of the ion exchange of Cd2+ into
 Ag+ beta-alumina
;
_journal_name_full               'Acta Crystallographica B (39,1983-)'
_journal_page_first              643
_journal_page_last               650
_journal_volume                  47
_journal_year                    1991
_chemical_formula_sum            'Ag1.12 Al11 Cd0.05 O17.11'
_chemical_name_systematic        'Ag1.12 Cd.05 Al11 O17.11'
_space_group_IT_number           194
_symmetry_space_group_name_Hall  '-P 6c 2c'
_symmetry_space_group_name_H-M   'P 63/m m c'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            2
_cell_length_a                   5.6032
_cell_length_b                   5.6032
_cell_length_c                   22.504
_cell_volume                     611.875
_citation_journal_id_ASTM        ASBSDK
_cod_data_source_file            silver1-2_580.cif
_cod_data_source_block           Ag1.12Al11Cd0.05O17.11
_cod_original_cell_volume        611.8748
_cod_database_code               2105353
Verbindungen mit Schichtstrukturen in den Systemen (Cu Ga5 S8)/ (Cu In5 S8) und (Ag Ga5 S8)/(Ag In5 S8)
Arzani, R.; Memo, A.; Elitok, E.; Haeuseler, H.; Zeitschrift fuer Anorganische und Allgemeine Chemie 627 (2001) 1204–1208; doi:10.1002/1521-3749(200106)627:6<1204::AID-ZAAC1204>3.0.CO;2-V

data_1509581
_publ_section_title
;
 Verbindungen mit Schichtstrukturen in den Systemen (Cu Ga5 S8)/ (Cu In5
 S8) und (Ag Ga5 S8)/(Ag In5 S8)
;
_journal_name_full
'Zeitschrift fuer Anorganische und Allgemeine Chemie'
_journal_page_first              1204
_journal_page_last               1208
_journal_paper_doi
10.1002/1521-3749(200106)627:6<1204::AID-ZAAC1204>3.0.CO;2-V
_journal_volume                  627
_journal_year                    2001
_chemical_formula_sum            'Ag1.12 Ga2.68 In3.7 S10'
_space_group_IT_number           186
_symmetry_space_group_name_Hall  'P 6c -2c'
_symmetry_space_group_name_H-M   'P 63 m c'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            1
_cell_length_a                   3.833
_cell_length_b                   3.833
_cell_length_c                   30.953
_cell_volume                     393.832
_citation_journal_id_ASTM        ZAACAB
_cod_data_source_file            silver1-2_581.cif
_cod_data_source_block           Ag1.12Ga2.68In3.7S10
_cod_database_code               1509581
Structural studies of stacking variants in Mg-base Friauf-Laves-phases
Komura, Y.; Tokunaga, K.; Acta Crystallographica B (24,1968-38,1982) 36 (1980) 1548–1554; doi:10.1107/S0567740880006565

data_2105354
_publ_section_title
;
 Structural studies of stacking variants in Mg-base Friauf-Laves-phases
;
_journal_name_full               'Acta Crystallographica B (24,1968-38,1982)'
_journal_page_first              1548
_journal_page_last               1554
_journal_paper_doi               10.1107/S0567740880006565
_journal_volume                  36
_journal_year                    1980
_chemical_formula_sum            'Ag1.15 Mg9 Zn16.85'
_space_group_IT_number           166
_symmetry_space_group_name_Hall  '-R 3 2"'
_symmetry_space_group_name_H-M   'R -3 m :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            2
_cell_length_a                   5.21
_cell_length_b                   5.21
_cell_length_c                   38.7
_cell_volume                     909.739
_citation_journal_id_ASTM        ACBCAR
_cod_data_source_file            silver1-2_582.cif
_cod_data_source_block           Ag1.15Mg9Zn16.85
_cod_original_cell_volume        909.7395
_cod_database_code               2105354
Impact of liquid quenching on aluminium-silver alloys
Anantharaman, T.R.; Ramachandrarao, P.; Current Science 37 (1968) 124–126; doi:

data_1509582
_publ_section_title
;
 Impact of liquid quenching on aluminium-silver alloys
;
_journal_name_full               'Current Science'
_journal_page_first              124
_journal_page_last               126
_journal_volume                  37
_journal_year                    1968
_chemical_formula_sum            'Ag1.2 Al2.8'
_chemical_name_systematic        '(Ag3 Al7)0.4'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            1
_cell_length_a                   4.0523
_cell_length_b                   4.0523
_cell_length_c                   4.0523
_cell_volume                     66.543
_citation_journal_id_ASTM        CUSCAM
_cod_data_source_file            silver1-2_583.cif
_cod_data_source_block           Ag1.2Al2.8
_cod_original_cell_volume        66.54337
_cod_database_code               1509582
Ca Ag - Sr Ag - Ba Ag: Between CrB and FeB structure type
Roehr, C.; Burggraf, F.; Duerr, I.; Harms, W.; Daub, M.; Zeitschrift fuer Anorganische und Allgemeine Chemie 634 (2008) 2255–2266; doi:

data_1509583
_publ_section_title
;
 Ca Ag - Sr Ag - Ba Ag: Between CrB and FeB structure type
;
_journal_name_full
'Zeitschrift fuer Anorganische und Allgemeine Chemie'
_journal_page_first              2255
_journal_page_last               2266
_journal_volume                  634
_journal_year                    2008
_chemical_formula_sum            'Ag1.2 Ca0.3 Sr0.9'
_chemical_name_systematic        'Sr0.9 Ca0.3 Ag1.2'
_space_group_IT_number           62
_symmetry_space_group_name_Hall  '-P 2ac 2n'
_symmetry_space_group_name_H-M   'P n m a'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            10
_cell_length_a                   24.3467
_cell_length_b                   4.7397
_cell_length_c                   6.292
_cell_volume                     726.072
_citation_journal_id_ASTM        ZAACAB
_cod_data_source_file            silver1-2_584.cif
_cod_data_source_block           Ag1.2Ca0.3Sr0.9
_cod_database_code               1509583
Ag1.2 V3 O8 crystal structure: relationship with Ag2 V4 O11-y and interpretation of physical properties
Rozier, P.; Galy, J.; Journal of Solid State Chemistry 134 (1997) 294–301; doi:10.1006/jssc.1997.7559

data_1509584
_publ_section_title
;
 Ag1.2 V3 O8 crystal structure: relationship with Ag2 V4 O11-y and
 interpretation of physical properties
;
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              294
_journal_page_last               301
_journal_paper_doi               10.1006/jssc.1997.7559
_journal_volume                  134
_journal_year                    1997
_chemical_formula_sum            'Ag1.2 O8 V3'
_chemical_name_systematic        'Ag1.2 (V3 O8)'
_space_group_IT_number           11
_symmetry_space_group_name_Hall  '-P 2yb'
_symmetry_space_group_name_H-M   'P 1 21/m 1'
_cell_angle_alpha                90
_cell_angle_beta                 107.39
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   7.382
_cell_length_b                   3.6029
_cell_length_c                   12.193
_cell_volume                     309.470
_citation_journal_id_ASTM        JSSCBI
_cod_data_source_file            silver1-2_585.cif
_cod_data_source_block           Ag1.2O8V3
_cod_original_cell_volume        309.4698
_cod_database_code               1509584
A single-crystal x-ray diffraction study of the ion exchange of Cd2+ into Ag+ beta-alumina
Edstroem, K.; Thomas, J.O.; Farrington, G.C.; Acta Crystallographica B (39,1983-) 47 (1991) 643–650; doi:

data_2105355
_publ_section_title
;
 A single-crystal x-ray diffraction study of the ion exchange of Cd2+ into
 Ag+ beta-alumina
;
_journal_name_full               'Acta Crystallographica B (39,1983-)'
_journal_page_first              643
_journal_page_last               650
_journal_volume                  47
_journal_year                    1991
_chemical_formula_sum            'Ag1.22 Al11 O17.11'
_space_group_IT_number           194
_symmetry_space_group_name_Hall  '-P 6c 2c'
_symmetry_space_group_name_H-M   'P 63/m m c'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            2
_cell_length_a                   5.5914
_cell_length_b                   5.5914
_cell_length_c                   22.43
_cell_volume                     607.297
_citation_journal_id_ASTM        ASBSDK
_cod_data_source_file            silver1-2_586.cif
_cod_data_source_block           Ag1.22Al11O17.11
_cod_original_cell_volume        607.2969
_cod_database_code               2105355
Homologous silver bismuth chalcogenide halides (N,x)P.I. syntheses and crystal structures of the (0,1)P compound Ag Bi2 S2 Cl3 and of three members of the (1,x)P solid solution series Ag(x) Bi(4-2x) S(6-4x) Br(4x)
Soehnel, T.; Ruck, M.; Poudeu Poudeu, P.F.; Zeitschrift fuer Anorganische und Allgemeine Chemie 630 (2004) 1276–1285; doi:10.1002/zaac.200400131

data_1509585
_publ_section_title
;
 Homologous silver bismuth chalcogenide halides (N,x)P.I. syntheses and
 crystal structures of the (0,1)P compound Ag Bi2 S2 Cl3 and of three
 members of the (1,x)P solid solution series Ag(x) Bi(4-2x) S(6-4x) Br(4x)
;
_journal_name_full
'Zeitschrift fuer Anorganische und Allgemeine Chemie'
_journal_page_first              1276
_journal_page_last               1285
_journal_paper_doi               10.1002/zaac.200400131
_journal_volume                  630
_journal_year                    2004
_chemical_formula_sum            'Ag1.27 Bi2.73 Br2.54 S3.46'
_space_group_IT_number           12
_symmetry_space_group_name_Hall  '-C 2y'
_symmetry_space_group_name_H-M   'C 1 2/m 1'
_cell_angle_alpha                90
_cell_angle_beta                 90.9
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   13.289
_cell_length_b                   4.085
_cell_length_c                   9.734
_cell_volume                     528.351
_citation_journal_id_ASTM        ZAACAB
_cod_data_source_file            silver1-2_587.cif
_cod_data_source_block           Ag1.27Bi2.73Br2.54S3.46
_cod_original_cell_volume        528.3505
_cod_database_code               1509585
Cs Fex Ag2-x Te2 (x=0.72): the first quaternary iron telluride synthesized from molten salt
Yglesias, R.A.; Guo, H.-Y.; Li, J.; Emge, T.J.; Chemistry of Materials (1,1989-) 7 (1995) 599–601; doi:

data_4001724
_publ_section_title
;
 Cs Fex Ag2-x Te2 (x=0.72): the first quaternary iron telluride
 synthesized from molten salt
;
_journal_name_full               'Chemistry of Materials (1,1989-)'
_journal_page_first              599
_journal_page_last               601
_journal_volume                  7
_journal_year                    1995
_chemical_formula_sum            'Ag1.28 Cs Fe0.72 Te2'
_chemical_name_systematic        'Cs Fe0.72 Ag1.28 Te2'
_space_group_IT_number           139
_symmetry_space_group_name_Hall  '-I 4 2'
_symmetry_space_group_name_H-M   'I 4/m m m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   4.5058
_cell_length_b                   4.5058
_cell_length_c                   15.4587
_cell_volume                     313.846
_citation_journal_id_ASTM        CMATEX
_cod_data_source_file            silver1-2_588.cif
_cod_data_source_block           Ag1.28Cs1Fe0.72Te2
_cod_original_cell_volume        313.8461
_cod_original_formula_sum        'Ag1.28 Cs1 Fe0.72 Te2'
_cod_database_code               4001724
Ternary gallides RE Agx Ga4-x (RE= La, Ce, Pr, Nd, Sm)
Hiebl, K.; Grin', Yu.N.; Rogl, P.; Eibler, R.; Journal of the Less-Common Metals 115 (1986) 367–372; doi:10.1016/0022-5088(86)90160-8

data_1509586
_publ_section_title
;
 Ternary gallides RE Agx Ga4-x (RE= La, Ce, Pr, Nd, Sm)
;
_journal_name_full               'Journal of the Less-Common Metals'
_journal_page_first              367
_journal_page_last               372
_journal_paper_doi               10.1016/0022-5088(86)90160-8
_journal_volume                  115
_journal_year                    1986
_chemical_formula_sum            'Ag1.296 Ce2 Ga6.704'
_chemical_name_systematic        '(Ag1.296 Ga6.704) Ce2'
_space_group_IT_number           139
_symmetry_space_group_name_Hall  '-I 4 2'
_symmetry_space_group_name_H-M   'I 4/m m m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            1
_cell_length_a                   4.318
_cell_length_b                   4.318
_cell_length_c                   10.737
_cell_volume                     200.193
_citation_journal_id_ASTM        JCOMAH
_cod_data_source_file            silver1-2_589.cif
_cod_data_source_block           Ag1.296Ce2Ga6.704
_cod_original_cell_volume        200.1927
_cod_database_code               1509586
Ternary gallides RE Agx Ga4-x (RE= La, Ce, Pr, Nd, Sm)
Hiebl, K.; Eibler, R.; Rogl, P.; Grin', Yu.N.; Journal of the Less-Common Metals 115 (1986) 367–372; doi:10.1016/0022-5088(86)90160-8

data_1509587
_publ_section_title
;
 Ternary gallides RE Agx Ga4-x (RE= La, Ce, Pr, Nd, Sm)
;
_journal_name_full               'Journal of the Less-Common Metals'
_journal_page_first              367
_journal_page_last               372
_journal_paper_doi               10.1016/0022-5088(86)90160-8
_journal_volume                  115
_journal_year                    1986
_chemical_formula_sum            'Ag1.296 Ga6.704 La2'
_chemical_name_systematic        '(Ag1.296 Ga6.704) La2'
_space_group_IT_number           139
_symmetry_space_group_name_Hall  '-I 4 2'
_symmetry_space_group_name_H-M   'I 4/m m m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            1
_cell_length_a                   4.361
_cell_length_b                   4.361
_cell_length_c                   10.715
_cell_volume                     203.781
_citation_journal_id_ASTM        JCOMAH
_cod_data_source_file            silver1-2_590.cif
_cod_data_source_block           Ag1.296Ga6.704La2
_cod_original_cell_volume        203.7813
_cod_database_code               1509587